# 4102- Chap 4 Fatigue.pdf

Embed Size (px)

### Transcript of 4102- Chap 4 Fatigue.pdf

MAAE 4012Strength & Fracture Analysis

Chapter 4

FatigueFatigue

Professor R. BellDepartment of Mechanical & Aerospace Engineering

Carleton University

© 2013

Chapter 4 - Fatigue 1

Crack Growth and FractureDepartment of Mechanical & Aerospace Engineering

Crack Growth takes place by:

Fatigue due to cyclic loading Stress Corrosion due to sustained loading C t t l di t hi h t t Creep - constant loading at high temperature Hydrogen induced cracking - Delayed hydride

cracking Liquid metal induced cracking. (of little interest in load

bearing structures. e.g. Hg in contact with Al)

Items 1 and 2 are of most interest in general design

Chapter 4 - Fatigue 2

DefinitionsDepartment of Mechanical & Aerospace Engineering

F ti i th t i t t k th h i

Fatigue

Fatigue is the most important crack growth mechanism Fatigue is a process of crack growth which causes damage

to a component subjected to repeated loading. This damage may result in final failuremay result in final failure.

Fatigue is a complex metallurgical process which is difficult to accurately describe

Assessment for fatigue in design must be made Assessment for fatigue in design must be made Fatigue can be divided into two periods

Initiation Propagation Propagation

Total Life (NT) = Initiation Life (Ni) + Propagation Life (Np)

Chapter 4 - Fatigue 3

Fatigue Design CriteriaDepartment of Mechanical

& Aerospace Engineering

Infinite Life design

Safe Life Design

Fail - Safe Design

Damage Tolerant Design

Chapter 4 - Introduction 4

Fatigue Design CriteriaDepartment of Mechanical

& Aerospace Engineering

Infinite Life Design Infinite Life Design Unlimited safety - requires design stresses to be safely

below the fatigue limit

Safe Life Design Designing for a finite life - Failure will not occur during

the life of the component. Safe life design must include a margin for the scatter of

fatigue results.Margin of safety = 20 x desired life e.g. pressure vessels and jet engines Landing gear are designed for safe life

Chapter 4 - Introduction 5

Fatigue Design CriteriaDepartment of Mechanical

& Aerospace Engineering

F il S f D i Fail - Safe Design

designed by aircraft engineers who could not tolerate extra weight required by large safety factors nor the danger resulting from small safety factors

Unlimited safety - requires design stresses to be safely below the fatigue limit

multiple load paths and crack arresters Aero engines are fail - safe designs only in multi-engine g g y g

aircraft

Chapter 4 - Introduction 6

Fatigue Design CriteriaDepartment of Mechanical

& Aerospace Engineering

D T l D i Damage Tolerant Design

Refinement of fail - safe philosophy Assumes that cracks exist and uses a Fracture

Mechanics analysis to check whether such cracks will grow large enough (critical size) to produce failures before they are sure to be detected and repaired

In pressure vessels "leak before burst" is an example of this philosophy

In aircraft – multiple load paths, crack arresters etc.

Chapter 4 - Introduction 7

Damage Tolerant DesignDepartment of Mechanical

& Aerospace Engineering

Philosophy Based on:

Damage will occur despite all precautions taken

Philosophy Based on:

Inspection so that cracks can be detected and repairs made at proper time

Adequate residual strength is maintained in the damaged structure so that during the period between inspections when the damage is undetected ultimateinspections when the damage is undetected ultimate failure of the structure is not possible.

Chapter 4 - Introduction 8

Fatigue Design MethodsDepartment of Mechanical & Aerospace Engineering

Stress Life Approach. – Total Life

Strain Life Approach. - Initiation Life Strain Life Approach. Initiation Life

Fracture Mechanics Approach – Propagation Life

Chapter 4 - Fatigue 9

Stress Life ApproachDepartment of Mechanical & Aerospace Engineering

Stress Life Approach Stress Life Approach

First fatigue method to be developed

Used mainly for long life applications were stresses and strains are elastic

It does not distinguish between initiation and propagation, but with the total life of a component. It deals with the life to failure of a component.

Chapter 4 - Fatigue 10

Strain Life ApproachDepartment of Mechanical & Aerospace Engineering

Strain Life Approach

Developed in the 1960's . This method is considered an initiation approach.

It is used when the strain is no longer totally elastic, but has a plastic component.

Short low cycle fatigue lives generally occur under these conditions.

Chapter 4 - Fatigue 11

Fracture Mechanics ApproachDepartment of Mechanical & Aerospace Engineering

Fracture Mechanics Approach

This method is based upon linear elastic fracture mechanics (LEFM) principles which are adapted for cyclic loading.

This method is used to predict propagation life f i iti l k d f tfrom an initial crack or defect.

This method is also used in combination with the strain life approach to predict the total lifestrain life approach to predict the total life (initiation and propagation).

Chapter 4 - Fatigue 12

Fatigue Limit – Ferrous Materials

Department of Mechanical &Aerospace Engineering

Fatigue Limit Ferrous Materials

F il t t ll b l th Failure at stresses well below the nominal tensile strength

50-90% of al structural failures occur by fatigue

Endurance – No of cycles to failure Most ferrous materials exhibit a Fatigue

Limit

Wohler carried out the first systematic test of railway axles under repeated loads in Germany in 1840’s

Analysis based on Wohler S-N Fatigue Limit

Stress level below which failure will not occur by fatigue

Fatigue Limit can disappear due to

Analysis based on Wohler S N diagram

Showed that fatigue life decreased with higher stress amplitudes

Fatigue Limit can disappear due to Periodic overloads Corrosive environments High temperatures

Chapter 4 - Fatigue 13

g p

Fatigue Limit – Non-Ferrous MaterialsDepartment of Mechanical &Aerospace Engineering

Non-Ferrous Materials Effect of Notches

Most Non-Ferrous materials have no fatigue / endurance limit

The presence of notches reduces the fatigue performance of material and structures

A Pseudo endurance limit is taken as the stress corresponding to a life of 5 x 108

cycles

structures

Chapter 4 - Fatigue 14

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Stress FluctuationMean Stress EffectMean Stress Effect Size Effect Surface Finish S f T t t Surface TreatmentPlatingThermalMechanical

Temperature Environment Environment Stress Concentration Kt

Chapter 4 - Fatigue 15

Stress FluctuationDepartment of Mechanical &Aerospace Engineering

Variable Amplitude Loadingp g

However:Most tests are carried out at Constant Amplitude loading

Chapter 4 - Fatigue 16

Constant Amplitude LoadingDepartment of Mechanical &Aerospace Engineering

Stress ratio R = Smin / Smax

Mean stress Sm

Stress Amplitude SStress Amplitude Sa

Stress Range = Smax – Smin

Show diagram of Mean loads

Chapter 4 - Fatigue 17

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Stress FluctuationMean Stress EffectMean Stress Effect Size Effect Surface Finish S f T t t Surface TreatmentPlatingThermalMechanical

Temperature Environment Environment Stress Concentration Kt

Chapter 4 - Fatigue 18

Effect of Mean StressDepartment of Mechanical &Aerospace Engineering

Mean stress has an effect on fatigue life

The effect can be portrayed as a function p yof Smean and Sa

1234 mmmm

Chapter 4- Fatigue 19

Mean Stress EquationsDepartment of Mechanical &Aerospace Engineering

1 :Goodman U

m

e

a

SS

1 : Gerber 2

U

m

e

a

SS

1 : Morrow

1 : Soderberg

ma

Y

m

e

a

SS

SS

fe SS

a = fatigue strength in terms of stress amplitude where m 0Se = fatigue strength in terms of stress amplitude where m = 0m = mean stressSu = Ultimate strengthSy = Yield strength = true fracture strength

Chapter 4 - Fatigue 20

f = true fracture strength

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Stress FluctuationMean Stress EffectMean Stress Effect Size Effect Surface Finish Surface Treatment Surface TreatmentPlatingThermalMechanical

Temperature Environment Environment Stress Concentration Kt

Chapter 4 - Fatigue 21

Size EffectDepartment of Mechanical &Aerospace Engineering

Other things being equal, an i i ti i illincrease in section size will result in a decrease in fatigue life

Fatigue is controlled by g yweakest link of the material

Probability of weak link increases with volume

A larger component will have a A larger component will have a larger surface volume and therefore a larger surface area subjected to high stress

Chapter 4 - Fatigue 22

Size Effect in Large and Small SpecimensDepartment of Mechanical &Aerospace Engineering

Larger volume subjected to higher stress

Cracks initiate earlier and propagate faster

Chapter 4 - Fatigue 23

Size Effect in Welded SpecimensDepartment of Mechanical &Aerospace Engineering

Weld toe radius does not scale up

Therefore hot spot has a higher local stress

Chapter 4 - Fatigue 24

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Factors that Influence Fatigue

Stress Fluctuation Stress FluctuationMean Stress Effect Size Effect Surface Finish Surface Finish Surface TreatmentPlatingThermalMechanical

Temperaturee pe atu e Environment Stress Concentration Kt

Chapter 4 - Fatigue 25

Surface FinishDepartment of Mechanical &Aerospace Engineering

Machining marks, scratches and surface scale lead to the initiation of cracks

The condition of the surface is more important for higher strength steels

Residual surface stresses caused by machining operation Residual surface stresses caused by machining operation can be important. An example can be the tensile residual stresses left by some grinding operations

At shorter lives where crack propagation dominates the At shorter lives, where crack propagation dominates, the condition of the surface finish has less effect on the fatigue life.

Localized surface irregularities such as stamping marks can Localized surface irregularities such as stamping marks can serve as very effective stress concentrations and should not be ignored.

Chapter 4 - Fatigue 26

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Factors that Influence Fatigue

Stress Fluctuation Stress FluctuationMean Stress Effect Size Effect Surface Finish Surface Finish Surface TreatmentPlatingThermalMechanical

Temperaturee pe atu e Environment Stress Concentration Kt

Chapter 4 - Fatigue 27

Surface TreatmentDepartment of Mechanical &Aerospace Engineering

Cracks initiate at the free surface therefore any surface treatment

Plating

has a significant effect

Chrome and Nickel plating can cause up to a 60% reduction in the endurance limit. Primarily due to the high residual tensile stresses caused by the plating processstresses caused by the plating process.

To alleviate the problem:-• Nitride part before plating• 2 Shot peen part before or after plating• 2. Shot peen part before or after plating• 3. Bake or anneal part after plating

Chapter 4 - Fatigue 28

Surface TreatmentDepartment of Mechanical &Aerospace Engineering

Thermal Treatment

Diffusion processes such as carburizing or nitriding. This process produces a higher strength material at the surface and

causes a volumetric change which produces residual compressive stresses.

Flame or Induction Hardening causes a phase transformation which produces a volumetric change causes a phase transformation which produces a volumetric change

which causes residual compressive stresses

Manufacturing processes such as welding, grinding and flame cuttingcutting can set up detrimental residual tensile stresses and shot peening can

undo some of this damage.

Chapter 4 - Fatigue 29

Surface TreatmentDepartment of Mechanical &Aerospace Engineering

Mechanical Treatment Cold working the surface can set up residual compressive Cold working the surface can set up residual compressive

stresses. Cold Rolling of screw threads Shot Peening Steel or glass beads fired at the surface to cause Shot Peening - Steel or glass beads fired at the surface to cause

yielding. Shot Peening has the greatest effect at long lives. Advantage - it can be applied to oddly shaped partsDisadvantage it dimples the surfaceDisadvantage - it dimples the surface At high temperatures the residual stresses can fade 500oF for steel and 250oF

for aluminium. Steels with yield stresses less than 80ksi are seldom cold rolled or shot

peened because with such low yield stresses it is possible to load to yield and wipe out the residual stresses.

Shot peening has the greatest effect when it is applied to areas of high stress gradients (i.e. at stress concentrations).

Chapter 4 - Fatigue 30

g ( )

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Factors that Influence Fatigue

Stress Fluctuation Stress FluctuationMean Stress Effect Size Effect Surface Finish Surface Finish Surface TreatmentPlatingThermalMechanical

Temperaturee pe atu e Environment Stress Concentration Kt

Chapter 4 - Fatigue 31

TemperatureDepartment of Mechanical &Aerospace Engineering

Temperature

At low temperature there is a tendency for the endurance p ylimits of steels to increase. However a more important design consideration is that the there is a significant decrease in fracture toughness at low temperatures

At high temperatures the endurance limit in steels disappearspp

At temperatures greater than 0.5 x the melting temperature creep becomes important. In this range the stress-lifecreep becomes important. In this range the stress life approach is no longer applicable.

Chapter 4- Fatigue 32

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Factors that Influence Fatigue

Temperaturee pe atu e Environment Stress Concentration Kt

Chapter 4 - Fatigue 33

EnvironmentDepartment of Mechanical &Aerospace Engineering

Environment

When fatigue loading takes place in a corrosive When fatigue loading takes place in a corrosive environment the net detrimental effect is more significant that if corrosion and fatigue were considered separately.

This is Corrosion Fatigue

Corrosion fatigue is not clearly understood - involves many variables

This topic will be considered later in course

Chapter 4 - Fatigue 34

Factors that Influence FatigueDepartment of Mechanical &Aerospace Engineering

Factors that Influence Fatigue

Temperaturee pe atu e Environment Stress Concentration Kt

Chapter 4 - Fatigue 35

Stress Concentration Factor Kt

Department of Mechanical &Aerospace Engineering

Stress Concentration Factor Kt

This is the ratio of the local to nominal stress Kt is too severe a factor where fatigue using the fatigue stress concentration factor Kf

KS

Sfe

un notched

enotched( )

( )K Kf t

e

qK f

1 q is the notch sensitivity factor which takes account ofq

K t

1factor which takes account of the sensitivity of the material to stress raisers

Chapter 4 - Fatigue 36

Stress Concentration Factor Kt

Department of Mechanical &Aerospace Engineering

Stress Concentration Factor Kt

1 N b1

Relationships for determining q

Peterson : q ar

1

1

Neuber : q

r

1

K 1K

Kar

ft

11

1

KK

r

ft

1

1

1

r

a = material constant aS k i

in

0 001

3001 8

..

Approximations for a for ferrous materials

r = notch root radius = material constant

S ksiU

aS MPa

mmU

0 025

20701 8

..

Chapter 4 - Fatigue 37

S MPaU

Stress Concentration Factor Kt

Department of Mechanical &Aerospace Engineering

Stress Concentration Factor Kt

Approximations for a for ferrous materials

aS ksi

inU

0 001

3001 8

..

aS MPa

mmU

0 025

20701 8

..

Using approximation Su 0.5 BHN

a for normalized or annealed steels 0.010 in (BHN 170)a for quenched and tempered steels 0.0025 in (BHN 360)a for highly hardened steels 0 001 in (BHN 600)a for highly hardened steels 0.001 in (BHN 600)

Chapter 4 - Fatigue 38

Notch Sensitivity CurvesDepartment of Mechanical &Aerospace Engineering

Notch Sensitivity Curves

PetersonNeuber

Chapter 4 - Fatigue 39

Neuber

Notch Sensitivity for Two Geometrically Similar Plates

Department of Mechanical &Aerospace Engineering

y y

Peterson : q a

1

1K

Kaf

t

1

1

1r 1

r 1

Approximations for a for ferrous materials

1 8.

aS ksi

inU

0 001

3001 8

..

Plate 1 Plate 2Plate 1 Plate 2

W1 = 5.0 in W2 = 0.5 ind1 = 0.5 in d2 = 0.05 inSu = 100 ksi Su = 100 ksiKt = 2.7 Kt = 2.7q = 0.97 q = 0.78Kf1 = 2 65 Kf2 = 2 32

Chapter 4 - Fatigue 40

Kf1 2.65 Kf2 2.32

Stress History or Cumulative Damage

Department of Mechanical &Aerospace Engineering

Stress History or Cumulative Damage

In most practical situations constant amplitude loading does not exist.

Stress Cycle Counting

The loading is variable amplitude

Stress Cycle Counting Cumulative Damage – Miner Summation This approach does not take account of the

order of stress cycles The order does have an effect on fatigue life

Chapter 4 - Fatigue 41

Miner Summation

Department of Mechanical &Aerospace Engineering

Miner Summation

nN

i

i 1

n n n nDi1 2 3

N N N NDamagei

i

1

1

2

2

3

3

Chapter 4 - Fatigue 42

Weld Detail ExampleDepartment of Mechanical &Aerospace Engineering

Offshore Detail F2 Classification

L S R Di ib iLong term Stress Range Distribution

Block Stress Range)Fi (MPa)

No of Cycles

NiNi

1 455 4

2 400 6

3 345 30

4 300 704 300 70

5 250 300

6 210 700

7 170 3,000

8 130 7,000

9 90 30,000

10 55 70,000

11 30 30,000

Chapter 4 - Fatigue 43

Weld Detail ExampleDepartment of Mechanical &Aerospace Engineering

Offshore Detail F2 Classification

The S-N curve for the F2 classification is:

tlog log log log

log . .

N am t

m

where a and m

4 22

1163 30

Determine the damage accumulation and hence estimate the cycles to failure

Chapter 4 - Fatigue 44

Weld Detail ExampleDepartment of Mechanical &Aerospace Engineering

Solution log log log logN am t

m 4 22

Block ni ∆i Ni ni/Ni

1 4 455 2924 0 0014

4 22log .

.

.log . logN 1163

304 0

4022

30

l lN 1144 30 1 4 455 2924 0.0014

2 6 400 4303 0.0014

3 30 345 6707 0.0045

4 70 300 10200 0.0069

log . . logN 1144 30

Total Damage D = 0.31515 300 250 17627 0.0170

6 700 210 29740 0.0235

7 3000 170 56060 0.0535

8 7000 130 125363 0.0558

No of cycles to failure

411110 9 30,000 90 377809 0.0794

10 70,000 55 1655434 0.0423

11 300,000 30 10200847 0.0294

ni = 411110 D = 0.3151

6103.13151.0

411110N

Chapter 4 - Fatigue 45

i

High / Low Cycle FatigueDepartment of Mechanical &Aerospace Engineering

High Cycle Fatigue Low Cycle Fatigue

Low stress levels High stress levels

High Cycle Fatigue Low Cycle Fatigue

Stress much less than yield

Cycles < 104

Cycles > 105

Chapter 4 - Fatigue 46

Strain Life Approach

Department of Mechanical &Aerospace Engineering

Strain Life Approach Strain life approach is based on observations of a component’s

response in critical regions (i e notches)response in critical regions (i.e. notches)

At high load levels in low cycle fatigue (LCF) regime the cyclic i d h i l b h i i bstress-strain response and the material behaviour is best

modelled by strain controlled conditions.

This method takes account of both elastic and plastic strains.

The strain-life approach assumes that smooth specimens tested pp punder strain controlled conditions can simulate the fatigue damage at the root of a notch.

Chapter 4 - Fatigue 47

Equally Stressed Volume of Material

Department of Mechanical &Aerospace Engineering

Equally Stressed Volume of Material Equivalent fatigue damage is assumed

to occur in the material at the notchto occur in the material at the notch root and in the smooth specimen when both are subjected to identical stress-strain histories.

Crack growth is not accounted for in this method.

Failure of the component is assumed Failure of the component is assumed to occur when the equally stressed volume fails.

This method is considered an This method is considered an initiation life estimate.

Chapter 4 - Fatigue 48

Fatigue Life PredictionDepartment of Mechanical &Aerospace Engineering

Fatigue Life PredictionTo predict fatigue life using the Strain – Life approach the following Information is required:

properties obtained from smooth specimen strain controlled fatigue data

the following Information is required:

specimen strain controlled fatigue data Stress-strain history at the critical

location e.g. at the notch Cycle counting information Cycle counting information Methods to incorporate mean stress

effects Damage summation techniques Damage summation techniques -

Miner's rule

Chapter 4 - Fatigue 49

Review of Monotonic Stress- Strain Behaviour

Department of Mechanical &Aerospace Engineering

SPA

Engineering Stress Aog g

Engineering Strain el

l

Engineering Strain e

lo

PTrue Stress

PA

dl ll

True Strain l lloo

ln

ln( )1 e S e( )1

Chapter 4 - Fatigue 50

( ) ( )

Cyclic Stress Strain BehaviourDepartment of Mechanical &Aerospace Engineering

is the total strain range is the total strain range is the total stress range

The total strain is the sum of th l ti d l ti t ithe elastic and plastic strains

amplitudesofin termspe

222

amplitudes of in terms

pe

The area within the loop is the energy dissipated during a cycle

Chapter 4 - Fatigue 51

Cyclic Strain Hardening and SofteningDepartment of Mechanical &Aerospace Engineering

D di th i iti l diti f t l d th t tDepending on the initial conditions of a metal and the test conditions, a metal may:

Cyclically hardeny y Cyclically soften Be cyclically stable Have mixed behaviour

(harden or soften depending on strain range)(harden or soften depending on strain range)

Chapter 4- Fatigue 52

Cyclic Strain Hardening and SofteningDepartment of Mechanical &Aerospace Engineering

Cyclic Hardening:"soft" material - initially dislocation so t ate a t a y d s ocat odensity is low - density increases due to cyclic plastic straining resulting in strain hardening

Cyclic Softening:"Hard" material - strain cycling y gcauses a rearrangement of dislocations which offers the least resistance to deformation

therefore the material softens- therefore the material softens

Chapter 4 - Fatigue 53

Cyclic Strain Hardening and SofteningDepartment of Mechanical &Aerospace Engineering

Strain Hardening and softening occurs during early fatigue life- then the material stabilizes - usually at about 20 - 40 % of the fatigue lifeTherefore fatigue properties are usually specified at half lifeg p p y p(at 50% of life when the material has stabilized)

Will Material Cyclically Harden Or Soften?

s 1.4 Material will cyclically hardenult

ult 12. Material will cyclically soften y

The monotonic strain hardening exponent n can also be used

n 0 2. Material will cyclically harden

n 01. Material will cyclically soften

Chapter 4 - Fatigue 54

Cyclic and Monotonic Stress-Strain CurvesDepartment of Mechanical &Aerospace Engineering

Chapter 4 - Fatigue 55

Strain – Life CurveDepartment of Mechanical &Aerospace Engineering

Basquin EquationBasquin (1910) observed that S-N data could be plotted on a log-log plot using true stress amplitude as:

22 f f

bN

Where:/2 = true stress amplitude2Nf = reversals to failure ( 2 rev = 1 cycle)'f = fatigue strength coefficientb f ti t th t (B i ' t)b = fatigue strength exponent (Basquins's exponent)'f is approximately equal to the true fracture strength fb is usually between -0.05 and -0.12

Manson Coffin EquationM d C ffi (19 0) f d h h Pl i i LifManson and Coffin (1950) found that the Plastic strain - Lifedata could also be linearized on a log-log plot.

c

Where:/2 = true strain amplitude2N l t f il ( 2 1 l )

2

2 f f

cN 2Nf = reversals to failure ( 2 rev = 1 cycle)

'f = fatigue ductility coefficientc = fatigue ductility exponent 'f is approximately equal to the true fracture ductility fc is usually between -0.5 and -0.7

Chapter 4 - Fatigue 56

y

Strain-Life RelationshipDepartment of Mechanical &Aerospace Engineering

Total Strain in terms of strain amplitude 2 2 2

e p

The elastic term can be written as: e

E2 2

In terms of life to failure (Basquin): 2

f bNIn terms of life to failure (Basquin): 2

2 fEN

Also the Plastic term is: (Manson-Coffin) p

f f

cN

22 2

Therefore the Total Strain can be written as:

22 2

f

f

b

f f

c

EN N

This is termed the Strain Life Relationshipat large strains or short lives plastic strain predominatesat small strains or short lives elastic strain predominates

Chapter 4 - Fatigue 57

Strain-Life RelationshipDepartment of Mechanical &Aerospace Engineering

Chapter 4 - Fatigue 58

Mean Stress EffectsDepartment of Mechanical &Aerospace Engineering

MORROW :Modify the elastic term

22 2

( )f of

b

f f

c

EN N 2 f f fE

-tensile mean stress-mean stress effect is significant at low values of plastic strain-predicts that the ratio of elastic to plastic strain depends on the stress ratio - this is not correct

Chapter 4 - Fatigue 59

Mean Stress EffectsDepartment of Mechanical &Aerospace Engineering

MANSON & HALFORD:

b

SMITH, WATSON & TOPPER (SWT)for completely reversed loading modified the strain life equation by the term

max 2

2f f

bN

multiplying the strain life equation by this term

( ) 22 f b b c

2

2 2

( )f of

b

ff o

f

cb

f

c

EN N

max

( )2

2 2 ff f f fE

N N

max is evaluated as o

2

Modified both the elastic and plastic terms to maintain the independence of the elastic / plastic ratio with mean Stress This approach tends to predict too much mean stress effect at short lives where the plastic strainspredominate

since max N f

when max < 0 this is undefinedTherefore this approach assumes that no fatigue damage occurs when < 0

Chapter 4 - Fatigue 60

predominate no fatigue damage occurs when max 0

Strain Life PredictionDepartment of Mechanical &Aerospace Engineering

Fatigue Analysis Procedure

ComponentGeometry

LoadingHistory

MaterialProperties

Stress-StrainAnalysis

Damage Analysis

Fatigue Life

Chapter 4 - Fatigue 61

Strain Life PredictionDepartment of Mechanical &Aerospace Engineering

The basic assumption of the strain-life (N) fatigue analysis approach is that fatigue damage accumulation and fatigue life to crack initiation at the notch tip, are the same as in a smooth material specimen, if subjected to the same stress-strain history.

Thus if the stress strain history at the notch tip of a machine Thus, if the stress-strain history at the notch tip of a machine component is the same as that one applied to a smooth specimen the fatigue life of the smooth laboratory specimen will be equal to the fatigue crack initiation life at the notch tipthe fatigue crack initiation life at the notch tip.

Chapter 4 - Fatigue 62

Smooth Specimen Notch TipDepartment of Mechanical &Aerospace Engineering

p p

peakS M

a)

peak

Stre

ss peak

Stre

ss

y y

x

y

x

x z

peakS M

Chapter 4 - Fatigue 63

Smooth Specimen Weld ToeDepartment of Mechanical &Aerospace Engineering

p

b)

Chapter 4 - Fatigue 64

Material Properties for -N ApproachDepartment of Mechanical &Aerospace Engineering

Stress – Strain Curve Strain – Life Curve

cbf NN 22 //

1

cff

bf

f NNE

222

/

'

'

n

E K

where: where:f ti t th ffi i tE – is the modulus of elasticity,

K’ – cyclic strength coefficient,n’ – strain hardening exponent

f’ - fatigue strength coefficient,b - fatigue strength exponent, f’ - fatigue ductility coefficient,c - fatigue ductility exponent

Chapter 4 - Fatigue 65

c at gue duct ty e po e t

Steps in a Fatigue Life PredictionDepartment of Mechanical &Aerospace Engineering

Analysis of external forces acting on the structure and the component in question (Fig. a, b),

Analysis of internal loads in chosen cross section of a component ( Analysis of internal loads in chosen cross section of a component ( Fig. b),

Selection of particular welded joints in the structure (Fig. c), Calculation of the peak stress, peak, at the critical point (Fig. d) Assembling of the stress peak history in the form of appropriate

sequence of stress peaks and valleys (Fig. e-f), Determination of the elastic-plastic response at the critical location

(Fig. h),(Fig. h), Identification (extraction) of cycles represented by closed stress-

strain hysteresis loops (Fig. i), Calculation of fatigue damage (Fig. j-k), Fatigue damage summation (Miner- Palmgren hypothesis, Fig. 4l), Determination of fatigue life (Fig. 4m) in terms of number of stress

history repetitions, Nblock, (No. of blocks) or the number of cycles to fatigue crack initiation, N.

Chapter 4 - Fatigue 66

fatigue crack initiation, N.

Steps in a Fatigue Life PredictionDepartment of Mechanical &Aerospace Engineering

a) Structure

Analysis of external f ti thforces acting on the structure

Analysis of internal loads in h

H

b) Component chosen cross section of a component

QF

Weld

c) Section with welded joint

Selection of

VP

R

peak

Selection of particular welded joints

Chapter 6 - Fatigue 67n

peak

hs

d)

Chapter 4 - Fatigue

Q

H

FSteps in a Fatigue Life predictionDepartment of Mechanical &Aerospace Engineering

Weld

c) Section with welded joint

VP

R

peak

n

peak

hs

h

d)

Calculation of the peak stress, peak, at the critical point using FE

nhsp g

analysis

Chapter 4 - Fatigue 68

Steps in a Fatigue Life predictionDepartment of Mechanical &Aerospace Engineering

1

e) g)

Assembling of the

0

'

'

n

E K

stress peak history

Determination of

1,1'1 1'

2

: peakNeuberE

f) h)

Determination of the elastic-plastic response at the critical location

35,5'

7,7'

pe

ak

t

1

2

35

7

2,2'

4

6

8

2

4

6

8

j)

Chapter 6 - Fatigue 69

''2 2

2bf

f f fN N cE

log

(/

2)

f

i)

Chapter 4 - Fatigue

5,5'

1,1'

ea

1 1'

2

: peakNeuberE

f) h)Steps in a Fatigue Life prediction

Department of Mechanical &Aerospace Engineering

35,5

7,7'

8

pe

k t

2

35

6

7

8

Identification of cycles represented b l d t 2,2'

4

6

4

6

'

'2 22

bff f fN N c

E

(/

2) fi)

j)

by closed stress-strain hysteresis loops

2 f f fE

/E

log

f/E

Calculation of fatigue damage

e/E

log (2Nf)0

2Ne2N

p e=

Fatigue damage:1 2 3 4 5

1 2 3 4 5

1 1 1 1 1; ; ; ; ;D D D D DN N N N N

k)

Total damage: 1 2 3 4 5 ;D D D D D D Fatigue life: N blck=1/Dl) j)

Fatigue damage by Miner summation

Chapter 4 - Fatigue 70

g 1 2 3 4 5 ;)

Fig. 4. (continued). Steps in fatigue life prediction procedure based on the -N approach

summation

Steps in a Fatigue Life PredictionDepartment of Mechanical &Aerospace Engineering

p g Analysis of external forces acting on the structure and the

component in question (Fig. a, b), Analysis of internal loads in chosen cross section of a component Analysis of internal loads in chosen cross section of a component

( Fig. b), Selection of particular welded joints in the structure (Fig. c), Calculation of the peak stress, peak, at the critical point (Fig. d) Assembling of the stress peak history in the form of appropriate

sequence of stress peaks and valleys (Fig. e-f), Determination of the elastic-plastic response at the critical location

(Fig. h),(Fig. h), Identification (extraction) of cycles represented by closed stress-

strain hysteresis loops (Fig. i), Calculation of fatigue damage (Fig. j-k), Fatigue damage summation (Miner- Palmgren hypothesis, Fig. l), Determination of fatigue life (Fig. m) in terms of number of stress

history repetitions, Nblock, (No. of blocks) or the number of cycles to fatigue crack initiation, N.

Chapter 4 - Fatigue 71

to fatigue crack initiation, N.

Factors Affecting Fatigue PerformanceDepartment of Mechanical &Aerospace Engineering

1. STRESS/LOAD State of Stress Stress Rangeg Stress Ratio Constant or Variable Loading Frequency Maximum Stress

2 GEOMETRY2. GEOMETRY Stress Raisers Size Stress Gradient Metallurgical & Mechanical 3 STAGES

Properties of Base Materials and Weldments

3. EXTERNAL ENVIRONMENT Temperature Aggressiveness

Fatigue Crack Initiation Fatigue Crack Propagation Final Failure - Fracture

Aggressiveness Corrosion Fatigue N N NT i p

Chapter 4 - Fatigue 72

Crack InitiationDepartment of Mechanical &Aerospace Engineering

CRACK INITIATIONat a surface - stress concentrations

f t h- surface scratches- dents- machining marks- fillets

SURFACE TREATMENTS1. MECHANICAL - Shot Peening

- Cold Rolling- Grinding- Polishing

2. THERMAL - Flame Hardening- Induction Hardening

3. SURFACE COATING- Nitriding- Plating

Chapter 4 - Fatigue 73

g

Crack GrowthDepartment of Mechanical &Aerospace Engineering

Crack Growth through loading and unloading cycle

Chapter 4 - Fatigue 74

Crack Growth and Stress Intensity FactorDepartment of Mechanical &Aerospace Engineering

maxmax

max

max

min 1

R

max1 R

K

aK

minmin

KKKR

max

min

aK

aK

maxmax

RKK

1max

This indicates that crack growth rate is a rising function of K and R.

),( RKfdNda

The process of crack growth is a complicated one,d it d dand it depends

on material behaviour therefore it is not possible to obtain this function

through rigorous mathematical description. It must be obtained from material tests, i.e. empirically.

Chapter 4 - Fatigue 75

, p y

Measurement of Growth Rate FunctionDepartment of Mechanical &Aerospace Engineering

For a wide plate with a small centre crack (a/W < 0.4, ≈ 1), aK

If the da/dN vs K results are plotted on a log-log plot the results are approximately a straight line of the form y= mx + C, i.e.

logloglog CKmdNda

Equation Paris theasknown is This

mKCdNda

dN

The values of C and m are obtained by curve fitting.

Chapter 4 - Fatigue 76

Measurement of Growth Rate FunctionDepartment of Mechanical &Aerospace Engineering

5

7

log40log)104log( :BPoint log3.6log)106.1log( :APoint

CmCm

38042log6.14.4log8.08.6

CmCm

310

10103.63.9log38.04.2

da

CCmm

310103.6 KdNda

where da/dN is in m/s and MPam

NOTE:The values of C and m depend on the units of the test data and conversion from one set of units to another should only be attempted with great caution.

Chapter 4 - Fatigue 77

Crack Propagation EquationsDepartment of Mechanical &Aerospace Engineering

PARIS EQUATIONdadN

C K m

FORMAN EQUATIONFORMAN EQUATIONThis equation shows the growth rate depends on R andalso at fracture when K =Kc the growth rate goes to 4

dadN

C KR K K

m

C

1

KLESNIL & LUKAS daC K Km m KLESNIL & LUKAS dNC K Km

thm

SCHULTZ

da C K Kmthm

dN R K KC

1

COLLIPRIEST

d K K R K Km

2 2 1ln

dadN

C K KKK

K R K KR K Kth

mc

th

C th

C th

2

2 11

exp ln arctanln

ln

Chapter 4 - Fatigue 78

Crack Propagation EquationsDepartment of Mechanical &Aerospace Engineering

STRESS INTENSITY FACTOR

MPa √m ksi √in Nmm-3/2 kp mm-3/2MPa √m ksi √in Nmm 3/2 kp mm 3/2

MPa √m 1 0.9101 31.623 3.2235

Ksi √in 1.0988 1 34.747 3.5420

N mm-3/2 0.031623 0.02878 1 0.10194

kp mm-3/2 0.31022 0.28233 9.8067 1

STRESS

MPa ksi N/mm2 kp/mm2

MPa 1 0.1449 1 0.1019

ksi 6 904 1 6 9033 0 7037ksi 6.904 1 6.9033 0.7037

N/mm2 1 0.1449 1 0.1019

kp/mm2 9.8067 1.4211 9.8067 1

Chapter 4 - Fatigue 79

Crack Propagation EquationsDepartment of Mechanical &Aerospace Engineering

The complete da/dN -K curve is sigmoidal in shape.

3 Regions Threshold P ti Propagation Fracture

Chapter 4 - Fatigue 80

Fatigue Crack ThresholdDepartment of Mechanical &Aerospace Engineering

Threshold Influenced by: Yield strength, grain size mean stress Stress History - residual stress C k ti i d Crack tip opening mode Temperature Environment

A lot of scatter in existing ΔKth datag Stress Ratio most important Factor

Estimates of ΔKthSteels: martensitic, bainetic, ferrite-pearlite, austeniticSteels: martensitic, bainetic, ferrite pearlite, austenitic

ΔKth = 6.4 (1 - 0.85 R)ksi √inR > + 1

ΔKth = 7 (1 - 0.85 R) MN/m3/2

ΔKth = 5.5 ksi √in constantR > 0.1

ΔKth = 6 MN/m3/2

Chapter 4 - Fatigue 81

Life Prediction – Constant Amplitude Loading

Department of Mechanical &Aerospace Engineering

d

ff aN

mKCdNda

Paris Equation

f

i

f a

am

N

Kda

CdN

0

1integrating

ff aN

m

dadN

aYK

1

ia

maYC

dN0

Chapter 4 - Fatigue 82

Life Prediction – Constant Amplitude

Department of Mechanical &Aerospace Engineering

p

Paris Equation – Closed form approach

a

m

da

KCdNda

f

q pp

12.1m

amf

aK

KdaN

i

SIF of an edge crack

0 12.1

1a

am

N

a

daC

dNf

i

f

g

22

22

11)12.1()2(

2m

f

m

i

mf

aaCmN

Integrating (for m 2)

Chapter 4 - Fatigue 83

fi

Life Prediction – Constant Amplitude

Department of Mechanical &Aerospace Engineering

Paris Equation – Closed form approach

22112

N f

q pp

22

22)12.1()2(

aaaCm m

f

m

i

mf Before this equation can be evaluated the final crack size must be calculated:

2

)( agfK

21

gfKa C

f

Chapter 4 - Fatigue 84

Life Prediction – ProcedureDepartment of Mechanical &Aerospace Engineering

1 Estimate the initial flaw size a1. Estimate the initial flaw size a02. Obtain SIF relationship3. Knowing KC or KIC and the nominal design stress -

Calculate the critical flaw size afCalculate the critical flaw size af4. Obtain the relationship relating da/dN with K e.g

1066.0 25.28 KdNda

I

5 Determine K for expression in (2)

inksiin isK and in/cyclein is dNdadN

5. Determine KI for expression in (2) 6. Integrate da/dN expression between limits a0 to af (at KIC)

to obtain life

Chapter 4 - Fatigue 85

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

1. AssumeA514 steelYS =100 ksi (689 MN/m2)K = 150 ksiin (165 MNm3/2)KIC = 150 ksiin (165 MNm3/2)a0 = 0.3 in (7.6 mm)Edge crack in tensiongmax = 45 ksi (310 MN/m2)max = 25 ksi (172 MN/m2) 20 k i (138 MN/ 2) = 20 ksi (138 MN/m2)

Chapter 4 - Fatigue 86

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

p

2. Edge crack in tension KI = 1.1.2 a3. Calculate the critical crack size aC at = 45 ksi

inKa ICcr 81.2

77.14512.1150

12.1

22

max

4. Assume an interval of crack growth – say a = 0.1 in (smaller intervals give slightly better results

5. Determine KI where aavg is the average crack size between ai and aj

Chapter 4 - Fatigue 87

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

p

6. Using the da/dN expression solve for N for each interval of crack growth a/N

Kdai1066.0 25.28

a

aN

KdN

avg

i

2098.11066.0

1066.0

25.28

7 Repeat for growth from 0 4 0 5 and so on

cyclesN

g

500,120.4 to0.3 fromgrowth crack For

7. Repeat for growth from 0.4 – 0.5 and so on.8. Total Life 86,700 cycles

Chapter 4 - Fatigue 88

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

p

ao af aavg )K )N GN)Ko

(in)f

(in)avg

(in) (ksi%in) (cycles) (cycles)

0.3 0.4 0.35 23.5 12,500 12,500

0.4 0.5 0.45 26.7 9,750 22,250

(ksi%in)

0.5 0.6 0.55 29.4 7,550 29,800

0.6 0.7 0.65 32.2 6,150 35,950

0.7 0.8 0.75 34.6 5,200 41,150Total Life

86 7000.8 0.9 0.85 36.6 4,600 45,750

0.9 1.0 0.95 38.8 4,100 49,850

1.0 1.1 1.05 40.5 3,700 53,550

86,700 cycles

1.1 1.2 1.15 42.5 3,300 56,850

1.2 1.3 1.25 44.5 2,950 59,800

1.3 1.4 1.35 46.1 2,700 62,500

Chapter 4 - Fatigue 89

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

p

Chapter 4 - Fatigue 90

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

p

1 I b i t h t i l i Hi h K

If the required Life is 100,000 cycles:Options:1. Increase af by using a tougher material i.e. Higher KIC2. Lower the design stress max i.e. Increase acrit at failure3. Lower stress

1. Decrease rate of crack growth2. Slightly lower has a significant effect on life due to

power law relationship

4. Improve fabrication quality and inspection capability so that the initial flaw size is reduced

Chapter 4 - Fatigue 91

Life Prediction – ExampleDepartment of Mechanical &Aerospace Engineering

If a0 were 0.2 in Total life = 104,700 cyclesIf a0 were 0.2 in Total life 104,700 cyclesN = 18,000 cycles for a = 0.2 0.3

Chapter 4 - Fatigue 92

Load Interaction - RetardationDepartment of Mechanical &Aerospace Engineering

Next Section

Chapter 4 - Fatigue 93

ReferencesDepartment of Mechanical &Aerospace Engineering

References N.E. Dowling, “Mechanical Behavior of Metals”, Prentice Hall, New

J 1999Jersey, 1999. A. Baumel and T. Seeger, “Materials Data for Cyclic Loading”,

Elsevier, Amsterdam, 1990. H Neuber “ Theory of Stress Concentration of Shear Strained H. Neuber, Theory of Stress Concentration of Shear Strained

Prismatic Bodies with Arbitrary Non Linear Stress-Strain Law”, ASME Journal of Applied Mechanics, vol. 28, 1961, pp. 544-550.

K. Molski and G. Glinka, “ A Method of ElasticPlastic Stress and K. Molski and G. Glinka, A Method of ElasticPlastic Stress and Strain Calculation at a Notch Root”, Material Science and Engineering, vol. 50, 1981, pp. 93-100.

A. Moftakhar, A. Buczynski and G. Glinka, “Calculation of Elasto-Plastic Strains and Stresses in Notches under Multiaxial Loading”, International Journal of Fracture, vol. 70, 1995, pp. 357-373.

Chapter 4 - Fatigue 94

ReferencesDepartment of Mechanical &Aerospace Engineering

J.M. Barsom and S.T. Rolfe,“Fatigue & Fracture Control in Structures”, Prentice Hall, 1987.

P.A. Ross-Ross, “Th I ti ti i t th C ki f P T b i Pi k i“The Investigation into the Cracking of Pressure Tubes in Pickering Units 3 and4”, From Steam to Space, CSME 1996.

“Standard Method for Plane-Strain Fracture Toughness of Metallic Materials”. ASTM Specification E-399-83p

Brock, D."Elementary Engineering Fracture Mechanics"(2nd Edition, Martinus Nijhoff Publishers, 1982)( , j , )

Brock, D."The Practrical Use of Fracture Mechanics“(Kluwer Academic Publishers, 1988)( , )

Anderson, T.L“Fracture Mechanics - Fundamentals and Applications”

(2 nd Edition, CRC Press, Boca Raton, 1995)

Chapter 4 - Fatigue 95

( d d t o , C C ess, oca ato , 995)

ReferencesDepartment of Mechanical &Aerospace Engineering

Bannantine, J.A., Comer, J.J. and Handrock, J.L. "Fundamental of Metal Fatigue Analysis“ (Prentice Hall, 1990)

Almar-Naess, A. "Fatigue Handbook - Offshore Steel structures“. (Tapir Publishers, Trondheim, Norway, 1985)

Chapter 4 - Fatigue 96